9/16/ :30 PM. Chapter 3. The structure of crystalline solids. Mohammad Suliman Abuhaiba, Ph.D., PE

Save this PDF as:

Size: px
Start display at page:

Transcription

1 Chapter 3 The structure of crystalline solids 1 Mohammad Suliman Abuhaiba, Ph.D., PE

2 2 Home Work Assignments HW 1 2, 7, 12, 17, 22, 29, 34, 39, 44, 48, 53, 58, 63 Due Sunday 17/9/2015

3 3 Why study the structure of crystalline solids? Properties of some materials are directly related to their crystal structure. Significant property differences exist between crystalline and noncrystalline materials having the same composition.

4 4 Crystal structures Fundamental concepts Crystalline materials: Atoms or ions form a regular repetitive, grid-like pattern, in 3D A lattice: collection of points called lattice points, arranged in a periodic pattern so that the surroundings of each point in the lattice are identical

5 5 Crystal structures Unit Cells Atoms arrange themselves into an ordered, 3d pattern called a crystal Unit cell (UC): smallest repeating volume within a crystal Each cell has all geometric features found in the total crystal

6 6 Metallic crystal structures Lattice Parameter: size & shape of UC, includes: 1. dimensions of sides of UC 2. angles between sides

7 7 Metallic crystal structures Face Centered Cubic (FCC) FCC: AL. Cu, Pb, Ag, Ni 4 atoms per unit cell Lattice parameter, a FCC Coordination Number (CN): # of atoms touching a particular atom, or # of nearest neighbors for that particular atom

8 8 Metallic crystal structures Face Centered Cubic (FCC) CN =12 APF = 0.74 Metals typically have relatively large APF to max shielding provided by the free electron cloud

9 9 Metallic crystal structures Face Centered Cubic (FCC)

10 10 Metallic crystal structures Example problem 3.1 Calculate 1. lattice parameter in terms of atomic radius R 2. volume of FCC UC in terms of R 3. atomic packing factor

11 11 Metallic crystal structures Body Centered Cubic (BCC) 2 atoms/uc Lattice parameter, a BCC CN = 8 APF = 0.68

12 12 Metallic Crystal Structures Hexagonal Closed-Packed Structure (HCP) c/a = No of atoms = 6 APF = 0.74

13 13 Density computation Density (No. of atoms/cell)(atomic mass) (volume of unit cell)(n ) (atoms)(g/mole) (cm )(atoms/mole) g cm 3 3 A

14 14 Density computation Example problem 3.2 Copper has an atomic radius of nm, an FCC crystal structure, and an atomic weight of 63.5 g/mol. Compute its theoretical density and compare the answer with its measured density.

15 15 Polymorphism and Allotropy Polymorphism: Materials that can have more than one crystal structure When found in pure elements condition is termed Allotropy A volume change may accompany transformation during heating or cooling. This volume change may cause brittle ceramic materials to crack and fail. Ex: Fe has BCC at RT which changes to FCC at 912 C

16 16 Crystal systems 7 possible systems (T3.2) and (F3.4).

17 17 Crystallographic Point Coordinates Point

18 18 Crystallographic Point Coordinates Example Problem 3.3 For the unit cell shown, locate the point having coordinates

19 19 Crystallographic Point Coordinates Example Problem 3.4 Specify point coordinates for all atom positions for a BCC UC.

20 20 Crystallographic Directions Metals deform in directions along which atoms are in closest contact. Many properties are directional. Miller indices are used to define directions.

21 21 Crystallographic Directions Procedure of finding Miller indices: RH coordinate system Find coordinates of 2 points along direction Subtract tail from head Clear fractions Enclose No s in [634] A direction and its ve are not identical A direction and its multiple are identical

22 22 Example Problem 3.5 Determine the indices for the direction shown in the figure.

23 23 Example Problem 3.6 Draw a direction within a cubic UC

24 24 Crystallographic Directions Families of directions Identical directions: any directional property will be identical in these directions Directions in cubic crystals having same indices without regard to order or sign are equivalent

25 25 Crystallographic Directions Miller-Bravais indices for hexagonal unit cells Directions in HCP: 3-axis or 4-axis system Move in each direction to get from tail to head of direction, while for consistency still making sure that u + v = -t

26 26 Crystallographic Directions Miller-Bravais indices for hexagonal unit cells Conversion from 3 axis to 4 axis: u = 1/3(2u` - v`) v = 1/3(2v` - u`) t = -(u + v) w = w` u`, v`, w`: indices in 3 axis system Clear fraction or reduce to lowest integer for values of u, v, t, and w.

27 27 Crystallographic Directions Example Problem 3.8 a) Convert [111] direction into four-index system for hexagonal crystals. b) Draw [111] direction within a HCP cell that utilizes a three-axis (a 1, a 2, z) coordinate system.

28 28 Example Problem 3.9 Determine the directional indices (fourindex system) for the direction shown.

29 29 Crystallographic planes Crystal contains planes of atoms that influence properties and behavior of a material. Metals deform along planes of atoms that are most tightly packed together. The surface energy of different faces of a crystal depends upon the particular crystallographic planes.

30 30 Crystallographic planes Calculation of planes Identify points at which plane intercepts x,y,z coordinates. If plane passes in origin of coordinates; system must be shifted. Take reciprocals of intercepts Clear fractions but do not reduce to lowest integer.

31 31 Crystallographic planes Calculation of planes Notes: Planes and their ve are identical Planes and their multiple are not identical For cubic crystals, planes and directions having the same indices are perpendicular to one another

32 32 Crystallographic planes Example Problem 3.10 Determine Miller indices for the plane shown in the figure.

33 33 Crystallographic planes Example Problem 3.11

34 34 Crystallographic planes Example Problem 3.12 Determine Miller Bravais indices for the plane shown in the hexagonal unit cell.

35 35 Crystallographic planes Atomic arrangements and Families of planes {} 2 or more planes may belong to same family of planes (same planner density) In cubic system only, planes having same indices irrespective of order & sign are equivalent. Ex: {111} is a family of planes that has 8 planes.

36 36 Linear and Planar Densities Repeat distance: distance between lattice points along the direction Repeating distance between equivalent sites differs from direction to direction. Ex: in the [111] of a BCC metal, lattice site is repeated every 2R. Ex: repeating distance in [110] for a BCC is, but for FCC.

37 37 Linear and Planar Densities Linear density: No of atoms per unit length along the direction. Equivalent directions have identical LDs In general, LD = 1 / repeat distance Example: find linear density along [110] for FCC. LD = number of atoms centered on direction vector length of direction vector

38 38 Linear and Planar Densities Planar packing fraction: fraction of area of the area of a plane actually covered by atoms In cubic systems, a direction that has the same indices as a plane is perpendicular to that plane. PD = number of atoms centered on a plane area of plane

39 39 Linear and Planar Densities PD = number of atoms centered on a plane area of plane

40 40 Linear and Planar Densities Ex: How many atoms per mm 2 are there on the (100) and (111) planes of lead (FCC) LD & PD are important considerations relative to the process of slip. Slip is the mechanism by which metals plastically deform Slip occurs on the most closely packed planes along directions having greatest LD

41 41 Crystallographic planes Closed Packed Planes and directions Close packed planes are (0001) & (0002) named basal planes. An HCP unit cell is built up by stacking together CPPs in a ABABAB stacking sequence.

42 42 Crystallographic planes Closed Packed Planes and directions Atoms in plane B (0002) fit into valleys between atoms on plane A (0001) Center atom in a basal plane is touched by: 6 atoms in same plane 3 atoms in a lower plane 3 atoms in upper plane CN =12

43 43 Crystallographic planes Closed Packed Planes and directions In FCC, CPPs are of the form {111} When parallel (111) planes are stacked: atoms in plane B fit over valleys in plane A atoms in plane C fit over valleys in both A & B 4 th plane fits directly over atoms in A A stacking sequence ABCABCABC is produced using (111) plane CN = 12

44 44 Crystallographic planes Closed Packed Planes and directions

45 45 Single Crystals Properties of single crystal materials depend upon chemical composition & specific directions within crystal Mohammad Suliman Abuhaiba, Ph.D., PE

46 46 Polycrystalline Materials Many properties of polycrystalline materials depend upon the physical and chemical char of both grains and grain boundaries.

47 47 Polycrystalline Materials Figure 3.18: stages in solidification of a polycrystalline material; square grids depict unit cells a) Small crystallite nuclei b) Growth of crystallites c) Upon completion of solidification, grains having irregular shapes have formed d) Grain structure as it would appear under the microscope; dark lines are grain boundaries

48 48 Polycrystalline Materials Figure 3.18

49 49 Anisotropy Anisotropic material: properties depend on the crystallographic direction along which the property is measured Isotropic material: properties are identical in all directions Most polycrystalline materials will exhibit isotropic properties. Table 3.3

50 50 Anisotropy

51 51 X-Ray Diffraction: Determination of Crystal Structures X-rays Electromagnetic radiation Wavelengths between 0.1Å & 100Å Similar to inter-atomic distances in a crystal

52 52 X-Ray Diffraction: Determination of Crystal Structures X-ray diffraction is a tool used to: 1. Identify phases by comparison with data from known structures 2. Quantify changes in cell parameters, orientation, crystallite size and other structural parameters 3. Determine crystallographic structure of novel or unknown crystalline materials.

53 53 X-Rray diffraction: Determination of Crystal Structures - Bragg s law An X-ray incident upon a sample will either: 1. Be transmitted: ray will continue along its original direction 2. Be scattered by electrons of the atoms in the material Interested in peaks formed when scattered X-rays constructively interfere.

54 54 X-Rray diffraction: Determination of Crystal Structures - Bragg s law Constructive Interference

55 55 X-Rray diffraction: Determination of Crystal Structures - Bragg s law Destructive Interference

56 56 X-Rray diffraction: Determination of Crystal Structures - Bragg s law Angle between transmitted & Bragg diffracted beams is always equal to 2θ This angle is readily obtainable in experimental situations Results of X-ray diffraction are frequently given in terms of 2θ

57 57 X-Rray diffraction: Determination of Crystal Structures - Bragg s law

58 58 X-RAY Diffraction: Determination of Crystal Structures - Inter-planar spacing Distance between adjacent parallel planes of atoms with the same Miller indices, d hkl In cubic cells, it s given by d hkl a o h k l

59 59 Example Calculate distance between adjacent (111) planes in gold which has a lattice constant of A.

60 60 X-RAY Diffraction: Determination of Crystal Structures - Powder diffraction A powder is a polycrystalline material There are all possible orientations of the crystals Similar planes in different crystals will scatter in different directions

61 61 X-RAY Diffraction: Determination of Crystal Structures - Powder diffraction In single crystal X-ray diffraction there is only one orientation. For a given wavelength & sample setting relatively few reflections can be measured: possibly zero, one or two As other crystals are added with slightly different orientations, several diffraction spots appear at the same 2θ value and spots start to appear at other values of 2θ.

62 62 X-RAY Diffraction: Determination of Crystal Structures - Powder diffraction Schematic diagram of an x-ray diffracto - meter T = x-ray source S = specimen C = detector O = axis of rotation of specimen & detector

63 63 X-RAY Diffraction: Determination of Crystal Structures - X-ray Diffractometer As the counter moves at constant angular velocity, a recorder automatically plots diffracted beam intensity as a function of 2q.

64 64 X-RAY Diffraction: Determination of Crystal Structures - X-ray Diffractometer Fig 3.22: a diffraction pattern for a powdered specimen High-intensity peaks result when Bragg diffraction condition is satisfied by some set of crystallographic planes. These peaks are plane-indexed in the figure

65 65 X-RAY Diffraction: Determination of Crystal Structures - X-ray Diffractometer Unit cell size & geometry may be resolved from angular positions of diffraction peaks Arrangement of atoms within unit cell is associated with relative intensities of these peaks.

66 66 X-RAY Diffraction: Determination of Crystal Structures Indexing Diffraction Pattern λ = 2 d sin θ d hkl a o h k l

67 67 Example Problem 3.13 For BCC iron, compute a. inter-planar spacing b. diffraction angle for (220) set of planes The lattice parameter for Fe is nm. Also, assume that monochromatic radiation having a wavelength of nm is used, and the order of reflection is 1.

Metallic crystal structures The atomic bonding is metallic and thus non-directional in nature

Chapter 3 The structure of crystalline solids Hw: 4, 6, 10, 14, 18, 21, 26, 31, 35, 39, 42, 43, 46, 48, 49, 51, 56, 61 Due Wensday 14/10/2009 Quiz1 on Wensday 14/10/2009 Why study the structure of crystalline

Introduction to Engineering Materials ENGR2000 Chapter 3: The Structure of Crystalline Solids. Dr. Coates

Introduction to Engineering Materials ENGR2000 Chapter 3: The Structure of Crystalline Solids Dr. Coates Learning Objectives I 1. Describe difference in atomic/molecular structure between crystalline/noncrystalline

Structure of silica glasses (Chapter 12)

Questions and Problems 97 Glass Ceramics (Structure) heat-treated so as to become crystalline in nature. The following concept map notes this relationship: Structure of noncrystalline solids (Chapter 3)

Chapter 3 Structure of Crystalline Solids

Chapter 3 Structure of Crystalline Solids Crystal Structures Points, Directions, and Planes Linear and Planar Densities X-ray Diffraction How do atoms assemble into solid structures? (for now, focus on

Fundamental concepts and language Unit cells Crystal structures! Face-centered cubic! Body-centered cubic! Hexagonal close-packed Close packed

Fundamental concepts and language Unit cells Crystal structures! Face-centered cubic! Body-centered cubic! Hexagonal close-packed Close packed crystal structures Density computations Crystal structure

Packing of atoms in solids

MME131: Lecture 6 Packing of atoms in solids A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s topics Atomic arrangements in solids Points, directions and planes in unit cell References:

Chapter Outline How do atoms arrange themselves to form solids?

Chapter Outline How do atoms arrange themselves to form solids? Fundamental concepts and language Unit cells Crystal structures Face-centered cubic Body-centered cubic Hexagonal close-packed Close packed

Carbon nanostructures. (http://www.mf.mpg.de/de/abteilungen/schuetz/index.php?lang=en&content=researchtopics&type=specific&name=h2storage)

Carbon nanostructures (http://www.mf.mpg.de/de/abteilungen/schuetz/index.php?lang=en&content=researchtopics&type=specific&name=h2storage) 1 Crystal Structures Crystalline Material: atoms arrange into a

STATE OF SOLIDIFICATION & CRYSTAL STRUCTURE

STATE OF SOLIDIFICATION & CRYSTAL STRUCTURE Chapter Outline Determination of crystal properties or properties of crystalline materials. Crystal Geometry! Crystal Directions! Linear Density of atoms! Crystal

Diffraction Basics. The qualitative basics:

The qualitative basics: Diffraction Basics Coherent scattering around atomic scattering centers occurs when x-rays interact with material In materials with a crystalline structure, x-rays scattered in

Energy and Packing. Materials and Packing

Energy and Packing Non dense, random packing Energy typical neighbor bond length typical neighbor bond energy r Dense, regular packing Energy typical neighbor bond length typical neighbor bond energy r

CHAPTER 3: CRYSTAL STRUCTURES & PROPERTIES

CHAPTER 3: CRYSTAL STRUCTURES & PROPERTIES ISSUES TO ADDRESS... How do atoms assemble into solid structures? (for now, focus on metals) How does the density of a material depend on its structure? When

UNIT V -CRYSTAL STRUCTURE

UNIT V -CRYSTAL STRUCTURE Solids are of two types: Amorphous and crystalline. In amorphous solids, there is no order in the arrangement of their constituent atoms (molecules). Hence no definite structure

Density Computations

CHAPTER 3 THE STRUCTURE OF CRYSTALLINE SOLIDS Fundamental Concepts 3.1 What is the difference between atomic structure and crystal structure? Unit Cells Metallic Crystal Structures 3.2 If the atomic radius

Two marks questions and answers. 1. what is a Crystal? (or) What are crystalline materials? Give examples

UNIT V CRYSTAL PHYSICS PART-A Two marks questions and answers 1. what is a Crystal? (or) What are crystalline materials? Give examples Crystalline solids (or) Crystals are those in which the constituent

Materials and their structures

Materials and their structures 2.1 Introduction: The ability of materials to undergo forming by different techniques is dependent on their structure and properties. Behavior of materials depends on their

Experiment 2b X-Ray Diffraction* Optical Diffraction Experiments

* Experiment 2b X-Ray Diffraction* Adapted from Teaching General Chemistry: A Materials Science Companion by A. B. Ellis et al.: ACS, Washington, DC (1993). Introduction Inorganic chemists, physicists,

ENGINEERING MATERIALS LECTURE #4

ENGINEERING MATERIALS LECTURE #4 Chapter 3: The Structure of Crystalline Solids Topics to Cover What is the difference in atomic arrangement between crystalline and noncrystalline solids? What features

11.3 The analysis of electron diffraction patterns

11.3 The analysis of electron diffraction patterns 277 diameter) Ewald reflecting sphere, the extension of the reciprocal lattice nodes and the slight buckling of the thin foil specimens all of which serve

Review of Metallic Structure

Phase Diagrams Understanding the Basics F.C. Campbell, editor Copyright 2012 ASM International All rights reserved www.asminternational.org Appendix A Review of Metallic Structure The word metal, derived

CRYSTAL LATTICE. Defining lattice: Mathematical construct; ideally infinite arrangement of points in space.

CRYSTAL LATTICE How to form a crystal? 1. Define the structure of the lattice 2. Define the lattice constant 3. Define the basis Defining lattice: Mathematical construct; ideally infinite arrangement of

CHAPTER 2. Structural Issues of Semiconductors

CHAPTER 2 Structural Issues of Semiconductors OUTLINE 1.0 Energy & Packing 2.0 Materials & Packing 3.0 Crystal Structures 4.0 Theoretical Density, r 5.0.Polymorphism and Allotropy 6.0 Close - Packed Crystal

Twins & Dislocations in HCP Textbook & Paper Reviews. Cindy Smith

Twins & Dislocations in HCP Textbook & Paper Reviews Cindy Smith Motivation Review: Outline Crystal lattices (fcc, bcc, hcp) Fcc vs. hcp stacking sequences Cubic {hkl} naming Hcp {hkil} naming Twinning

Review key concepts from last lecture (lattice + basis = unit cell) Bravais lattices Important crystal structures Intro to miller indices

Outline: Review key concepts from last lecture (lattice + basis = unit cell) Bravais lattices Important crystal structures Intro to miller indices Review (example with square lattice) Lattice: square,

Diffraction: Powder Method

Diffraction: Powder Method Diffraction Methods Diffraction can occur whenever Bragg s law λ = d sin θ is satisfied. With monochromatic x-rays and arbitrary setting of a single crystal in a beam generally

3.40 Sketch within a cubic unit cell the following planes: (a) (01 1 ) (b) (112 ) (c) (102 ) (d) (13 1) Solution

3.40 Sketch within a cubic unit cell the following planes: (a) (01 1 ) (b) (11 ) (c) (10 ) (d) (13 1) The planes called for are plotted in the cubic unit cells shown below. 3.41 Determine the Miller indices

Engineering Materials Department of Physics K L University

Engineering Materials Department of Physics K L University 1 Crystallography Bonding in solids Many of the physical properties of materials are predicated on a knowledge of the inter-atomic forces that

It is instructive however for you to do a simple structure by hand. Rocksalt Structure. Quite common in nature. KCl, NaCl, MgO

Today the structure determinations etc are all computer -assisted It is instructive however for you to do a simple structure by hand Rocksalt Structure Quite common in nature KCl, NaCl, MgO 9-1 Typical

Impurities in Solids. Crystal Electro- Element R% Structure negativity Valence

4-4 Impurities in Solids 4.4 In this problem we are asked to cite which of the elements listed form with Ni the three possible solid solution types. For complete substitutional solubility the following

X-ray diffraction and structure analysis Introduction

Teknillisen fysiikan ohjelmatyö X-ray diffraction and structure analysis Introduction Oleg Heczko 120 100 80 118 12-5 125 Ni-Mn-Ga (298K) SQRT(Intensity) 60 40 20 015 200 123 12-7 20-10 20,10 20-8 040

Basic Solid State Chemistry, 2 nd ed. West, A. R.

Basic Solid State Chemistry, 2 nd ed. West, A. R. Chapter 1 Crystal Structures Many of the properties and applications of crystalline inorganic materials revolve around a small number of structure types

3.091 Introduction to Solid State Chemistry. Lecture Notes No. 5 X-RAYS AND X-RAY DIFFRACTION

3.091 Introduction to Solid State Chemistry Lecture Notes No. 5 X-RAYS AND X-RAY DIFFRACTION * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * * Sources

Lecture # 11 References:

Lecture # 11 - Line defects (1-D) / Dislocations - Planer defects (2D) - Volume Defects - Burgers vector - Slip - Slip Systems in FCC crystals - Slip systems in HCP - Slip systems in BCC Dr.Haydar Al-Ethari

Engineering 45: Properties of Materials Final Exam May 9, 2012 Name: Student ID number:

Engineering 45: Properties of Materials Final Exam May 9, 2012 Name: Student ID number: Instructions: Answer all questions and show your work. You will not receive partial credit unless you show your work.

ENERGY AND PACKING. Chapter 3 CRYSTAL STRUCTURE & PROPERTIES MATERIALS AND PACKING METALLIC CRYSTALS ISSUES TO ADDRESS...

Chapter 3 CRYSTAL STRUCTURE & PROPERTIES ISSUES TO ADDRESS... 1. How do s assemble into solid structures? (For now, focus on metals) ENERGY AND PACKING non dense, random packing bond energy Energy bond

CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS

CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and Self-Interstitials 5.1 Calculate the fraction of atom sites that are vacant for copper at its melting temperature of 1084 C (1357 K). Assume

Chapter Outline Dislocations and Strengthening Mechanisms. Introduction

Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip

Earth & Planetary Science Applications of X-Ray Diffraction: Advances Available for Research with our New Systems

Earth & Planetary Science Applications of X-Ray Diffraction: Advances Available for Research with our New Systems James R. Connolly Dept. of Earth & Planetary Sciences University of New Mexico 401/501

3. Anisotropic blurring by dislocations

Dynamical Simulation of EBSD Patterns of Imperfect Crystals 1 G. Nolze 1, A. Winkelmann 2 1 Federal Institute for Materials Research and Testing (BAM), Berlin, Germany 2 Max-Planck- Institute of Microstructure

Travaux Pratiques de Matériaux de Construction

Travaux Pratiques de Matériaux de Construction Section Matériaux 6 ème semestre 2009 Etude de Matériaux Cimentaire Par Diffraction des Rayons X Responsable: Silke Ruffing E-Mail: silke.ruffing@epfl.ch

Symmetry in crystalline solids.

Symmetry in crystalline solids. Translation symmetry n 1,n 2,n 3 are integer numbers 1 Unitary or primitive cells 2D 3D Red, green and cyano depict all primitive (unitary) cells, whereas blue cell is not

High Resolution X-ray Diffraction

High Resolution X-ray Diffraction Nina Heinig with data from Dr. Zhihao Donovan Chen, Panalytical and slides from Colorado State University Outline Watlab s new tool: Panalytical MRD system Techniques:

CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS ev /atom = exp. kt ( =

CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and Self-Interstitials 5.1 Calculate the fraction of atom sites that are vacant for copper at its melting temperature of 1084 C (1357 K). Assume

Fundamentals of Plastic Deformation of Metals

We have finished chapters 1 5 of Callister s book. Now we will discuss chapter 10 of Callister s book Fundamentals of Plastic Deformation of Metals Chapter 10 of Callister s book 1 Elastic Deformation

CRYSTAL STRUCTURE, MECHANICAL BEHAVIOUR & FAILURE OF MATERIALS

MODULE ONE CRYSTAL STRUCTURE, MECHANICAL BEHAVIOUR & FAILURE OF MATERIALS CRYSTAL STRUCTURE Metallic crystal structures; BCC, FCC and HCP Coordination number and Atomic Packing Factor (APF) Crystal imperfections:

Point Defects in Metals

CHAPTER 5 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Point Defects in Metals 5.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 327 C (600 K). Assume an energy

Microstructural parameters from Multiple Whole Profile (MWP) or Convolutional Multiple Whole Profile (CMWP) computer programs

Microstructural parameters from Multiple Whole Profile (MWP) or Convolutional Multiple Whole Profile (CMWP) computer programs Iuliana Dragomir-Cernatescu School of Materials Science and Engineering, Georgia

Quiz on Monday covering: -symmetry operations -notations of axes, vectors, and face notation -Miller indices

OTHER ANNOUNCEMENTS Quiz on Monday covering: -symmetry operations -notations of axes, vectors, and face notation -Miller indices 2 nd Draft of References due Monday Field Trip Saturday 10/4 and Sunday

Primitive cells, Wigner-Seitz cells, and 2D lattices. 4P70, Solid State Physics Chris Wiebe

Primitive cells, Wigner-Seitz cells, and 2D lattices 4P70, Solid State Physics Chris Wiebe Choice of primitive cells! Which unit cell is a good choice?! A, B, and C are primitive unit cells. Why?! D, E,

An Introduction to X-Ray Powder Diffraction. credits to: Scott A Speakman, Patrick McArdle Edited by Di Cicco 2014

An Introduction to X-Ray Powder Diffraction credits to: Scott A Speakman, Patrick McArdle Edited by Di Cicco 2014 LATTICE ARRAYS AND BRAVAIS LATTICES Crystalline materials differ from amorphous materials

Travaux Pratiques de Matériaux de Construction. Etude de Matériaux Cimentaires par Diffraction des Rayons X sur Poudre

Travaux Pratiques de Matériaux de Construction Section Matériaux 6 ème semestre 2015 Etude de Matériaux Cimentaires par Diffraction des Rayons X sur Poudre Study Cementitious Materials by X-ray diffraction

A Brief History of XRD 1895: Röntgen discovers X-Rays received the first Nobel prize in physics in 1901

X-ray Diffraction A Brief History of XRD 1895: Röntgen discovers X-Rays received the first Nobel prize in physics in 1901 1912: Laue diffracts X-Rays from single crystal 1914 Nobel prize in Physics 1912:

X-Ray Diffraction Analysis

162402 Instrumental Methods of Analysis Unit III X-Ray Diffraction Analysis Dr. M. Subramanian Associate Professor Department of Chemical Engineering Sri Sivasubramaniya Nadar College of Engineering Kalavakkam

A - Transformation of anatase into rutile

Exercise-Course-XRD.doc 1/12 04/06/2012 A - Transformation of anatase into rutile Anatase and rutile are two distinct phases of titanium dioxide TiO 2. The stable phase is rutile. 1. Structural study Anatase:

1.10 Close packed structures cubic and hexagonal close packing

1.9 Description of crystal structures The most common way for describing crystal structure is to refer the structure to the unit cell. The structure is given by the size and shape of the cell and the position

Basic X-ray Powder Diffraction (XRPD)

Basic X-ray Powder Diffraction (XRPD) Solid-State, Material Science Crystalline (Scattering : diffraction) Non-crystalline (Scattering) Analytical Tool Qualitative and Quantitative Analysis Quantitative

AP 5301/8301 Instrumental Methods of Analysis and Laboratory Lecture 5 X ray diffraction

1 AP 5301/8301 Instrumental Methods of Analysis and Laboratory Lecture 5 X ray diffraction Prof YU Kin Man E-mail: kinmanyu@cityu.edu.hk Tel: 3442-7813 Office: P6422 Lecture 5: Outline Review on crystallography

TOPIC 2. STRUCTURE OF MATERIALS III

Universidad Carlos III de Madrid www.uc3m.es MATERIALS SCIENCE AND ENGINEERING TOPIC 2. STRUCTURE OF MATERIALS III Topic 2.3: Crystalline defects. Solid solutions. 1 PERFECT AND IMPERFECT CRYSTALS Perfect

Strengthening Mechanisms

Strengthening Mechanisms The ability of a metal/ alloy to plastically deform depends on the ability of dislocations to move. Strengthening techniques rely on restricting dislocation motion to render a

Rietveld refinement of ZrSiO 4 : application of a phenomenological model of anisotropic peak width

Rietveld refinement of ZrSiO 4 : application of a phenomenological model of anisotropic peak width A. Sarkar, P. Mukherjee, P. Barat Variable Energy Cyclotron Centre 1/A Bidhan Nagar, Kolkata 700064, India

Problem Set 2 Solutions

M 4733: Deformation and Fracture of ngineering Materials Spring 00 Problem Set Solutions *) Prove that for the case of cubic crystals the modulus of elasticity in any given direction may be given by the

EBSD Basics EBSD. Marco Cantoni 021/ Centre Interdisciplinaire de Microscopie Electronique CIME. Phosphor Screen. Pole piece.

EBSD Marco Cantoni 021/693.48.16 Centre Interdisciplinaire de Microscopie Electronique CIME EBSD Basics Quantitative, general microstructural characterization in the SEM Orientation measurements, phase

Stress-Strain Relationship and XRD Line Broadening in [0001] Textured Hexagonal Polycrystalline Materials

(Journal of the Society of Materials Science, Japan), Vol. 60, No. 7, pp. 642-647, July 2011 Original Papers Stress-Strain Relationship and XRD Line Broadening in [0001] Textured Hexagonal Polycrystalline

What if your diffractometer aligned itself?

Ultima IV Perhaps the greatest challenge facing X-ray diffractometer users today is how to minimize time and effort spent on reconfiguring of the system for different applications. Wade Adams, Ph.D., Director,

Phase Transformations in Metals Tuesday, December 24, 2013 Dr. Mohammad Suliman Abuhaiba, PE 1

Ferrite - BCC Martensite - BCT Fe 3 C (cementite)- orthorhombic Austenite - FCC Chapter 10 Phase Transformations in Metals Tuesday, December 24, 2013 Dr. Mohammad Suliman Abuhaiba, PE 1 Why do we study

a. 50% fine pearlite, 12.5% bainite, 37.5% martensite. 590 C for 5 seconds, 350 C for 50 seconds, cool to room temperature.

Final Exam Wednesday, March 21, noon to 3:00 pm (160 points total) 1. TTT Diagrams A U.S. steel producer has four quench baths, used to quench plates of eutectoid steel to 700 C, 590 C, 350 C, and 22 C

GEOLOGY 333 LAB 14. Lab Final Exam See information sheet for details

GEOLOGY 333 LAB 14 X-RAY DIFFRACTION OF EVERYDAY MATERIALS Lab Final Exam See information sheet for details! Next week during Lab (10 am - noon, May 2, 69 CAB).! 25% of Lab grade, out of 65 points plus

Lectures on: Introduction to and fundamentals of discrete dislocations and dislocation dynamics. Theoretical concepts and computational methods

Lectures on: Introduction to and fundamentals of discrete dislocations and dislocation dynamics. Theoretical concepts and computational methods Hussein M. Zbib School of Mechanical and Materials Engineering

Supplementary Figure 1: Geometry of the in situ tensile substrate. The dotted rectangle indicates the location where the TEM sample was placed.

Supplementary Figures Supplementary Figure 1: Geometry of the in situ tensile substrate. The dotted rectangle indicates the location where the TEM sample was placed. Supplementary Figure 2: The original

Measurement of Residual Stress by X-ray Diffraction

Measurement of Residual Stress by X-ray Diffraction C-563 Overview Definitions Origin Methods of determination of residual stresses Method of X-ray diffraction (details) References End Stress and Strain

Ph.D. Admission 20XX-XX Semester X Written Examination Materials Science & Engineering Department, IIT Kanpur Date of Examination: XX XXXX 20XX Timing: XX:XX XX:XX XX Application# Please read these instructions

EBSD Electron BackScatter Diffraction Principle and Applications

EBSD Electron BackScatter Diffraction Principle and Applications Dr. Emmanuelle Boehm-Courjault EPFL STI IMX Laboratoire de Simulation des Matériaux LSMX emmanuelle.boehm@epfl.ch 1 Outline! Introduction!

Transmission Electron Microscopy (TEM) Prof.Dr.Figen KAYA

Transmission Electron Microscopy (TEM) Prof.Dr.Figen KAYA Transmission Electron Microscope A transmission electron microscope, similar to a transmission light microscope, has the following components along

Bio5325 Fall Crystal Vocabulary

Crystals and Crystallization Bio5325 Fall 2007 Crystal Vocabulary Mosaicity (mosaic spread) Protein crystals are imperfect, consisting of a mosaic of domains that are slightly misaligned. As a result,

STRENGTHENING MECHANISM IN METALS

Background Knowledge Yield Strength STRENGTHENING MECHANISM IN METALS Metals yield when dislocations start to move (slip). Yield means permanently change shape. Slip Systems Slip plane: the plane on which

Formability and Crystallographic Texture in Novel Magnesium Alloys

Formability and Crystallographic Texture in Novel Magnesium Alloys Carlos Soto, Dr. Pnina Ari-Gur, Andreas, Quojo Quainoo, Dr. Betsy Aller, Dr. Andrew Kline Western Michigan University Abstract By looking

X-RAY POWDER DIFFRACTION XRD

X-RAY POWDER DIFFRACTION XRD for the analyst Getting acquainted with the principles Martin Ermrich nλ = 2d sin θ Detlef Opper The Analytical X-ray Company X-RAY POWDER DIFFRACTION XRD for the analyst Getting

Electron microscopy II

Electron microscopy II Nanomaterials characterization I RNDr. Věra Vodičková, PhD. Interaction ction: electrons solid matter Signal types SE.secondary e - AE Auger s e - BSE back scattered e - X-ray photons,

Basic Crystallography

Basic Crystallography Data collection and processing Louise N. Dawe, PhD Wilfrid Laurier University Department of Chemistry and Biochemistry References and Additional Resources Faculty of Science, Bijvoet

Small-angle X-ray scattering (SAXS) with synchrotron radiation

Small-angle X-ray scattering (SAXS) with synchrotron radiation Martin Müller Institut für Experimentelle und Angewandte Physik der Christian-Albrechts-Universität zu Kiel Introduction to small-angle scattering

Point Defects. Vacancies are the most important form. Vacancies Self-interstitials

Grain Boundaries 1 Point Defects 2 Point Defects A Point Defect is a crystalline defect associated with one or, at most, several atomic sites. These are defects at a single atom position. Vacancies Self-interstitials

Thin Film Scattering: Epitaxial Layers

Thin Film Scattering: Epitaxial Layers 6th Annual SSRL Workshop on Synchrotron X-ray Scattering Techniques in Materials and Environmental Sciences: Theory and Application May 29-31, 2012 Thin films. Epitaxial

Single-Crystal Plasticity

Single-Crystal Plasticity Eric M. Taleff, Department of Mechanical Engineering, Austin, TX 78712 October 10, 2005 Single-Crystal Plasticity p.1 Schmid Factor [uvw] σ applied λ θ (hkl) The relationship

Thin Film Characterizations Using XRD The Cases of VO2 and NbTiN

Thin Film Characterizations Using XRD The Cases of VO2 and NbTiN A thesis submitted in partial fulfillment of the requirement for the degree of Bachelor of Arts / Science in Physics from The College of

Learning Objectives. Chapter Outline. Solidification of Metals. Solidification of Metals

Learning Objectives Study the principles of solidification as they apply to pure metals. Examine the mechanisms by which solidification occurs. - Chapter Outline Importance of Solidification Nucleation

Module-6. Dislocations and Strengthening Mechanisms

Module-6 Dislocations and Strengthening Mechanisms Contents 1) Dislocations & Plastic deformation and Mechanisms of plastic deformation in metals 2) Strengthening mechanisms in metals 3) Recovery, Recrystallization

Steps in solving a structure. Diffraction experiment. Obtaining well-diffracting crystals. Three dimensional crystals

Protein structure from X-ray diffraction Diffraction images: ciprocal space Protein, chemical structure: IALEFGPSLKMNE Conformation, 3D-structure: CRYST1 221.200 73.600 80.900 90.00 90.00 90.00 P 21 21

Imaging with Diffraction Contrast

Imaging with Diffraction Contrast Duncan Alexander EPFL-CIME 1 Introduction When you study crystalline samples TEM image contrast is dominated by diffraction contrast. An objective aperture to select either

DIFFRACTION METHODS IN MATERIAL SCIENCE. PD Dr. Nikolay Zotov Tel Room 3N16.

DIFFRACTION METHODS IN MATERIAL SCIENCE PD Dr. Nikolay Zotov Tel. 0711 689 3325 Email: zotov@imw.uni-stuttgart.de Room 3N16 Lecture 7 OUTLINE OF THE COURSE 0. Introduction 1. Classification of Materials

E. Buffagni, C. Ferrari, L. Zanotti, A. Zappettini

E. Buffagni, C. Ferrari, L. Zanotti, A. Zappettini IMEM-CNR Institute, Parma (Italy) 1. Laue lenses for hard x-ray astronomy 2. Mosaic crystals 3. GaAs crystals 4. X-ray diffraction characterization 5.

GEOL.3070 EARTH MATERIALS I FORENSIC APPLICATIONS OF X-RAY DIFFRACTION

GEOL.3070 EARTH MATERIALS I FORENSIC APPLICATIONS OF X-RAY DIFFRACTION NAME I. Introduction Our knowledge of the crystalline state is gained by studies utilizing x-rays (the field of x- ray crystallography).

Condensed Matter II: Particle Size Broadening

Condensed Matter II: Particle Size Broadening Benjamen P. Reed & Liam S. Howard IMAPS, Aberystwyth University March 19, 2014 Abstract Particles of 355µm silicon oxide(quartz)were subjected to a ball milling

Dislocations and Plastic Deformation

Dislocations and Plastic Deformation Edge and screw are the two fundamental dislocation types. In an edge dislocation, localized lattice distortion exists along the end of an extra half-plane of atoms,

Kinematical theory of contrast

Kinematical theory of contrast Image interpretation in the EM the known distribution of the direct and/or diffracted beam on the lower surface of the crystal The image on the screen of an EM = the enlarged

Influence of Bulk Graphite Thickness on the Accuracy of X-Ray Diffraction Measurement. I. Introduction

Influence of Bulk Graphite Thickness on the Accuracy of X-Ray Diffraction Measurement Jane Y. Howe 1*, Burl O. Cavin 1, Amy E. Drakeford 2, Roberta A. Peascoe 1, Tracy L. Zontek 2, and Douglas J. Miller

CHAPTER 6: CRYSTAL GROWTH & XRD. Sarah Lambart

CHAPTER 6: CRYSTAL GROWTH & XRD Sarah Lambart RECAP CHAP. 5 (SEE REVIEW CHAPTER) Crystal twinning Crystal defects Polymorphism and isomorphism CONTENT CHAP. 6 (2 LECTURES) Part 1: Crystal growing - nucleation

Non-crystalline Materials

Noncrystalline (or amorphous) solids by definition means atoms are stacked in irregular, random patterns. The general term for non-crystallline solids with compositions comparable to those of crystalline

Instrument Configuration for Powder Diffraction

Instrument Configuration for Powder Diffraction Advanced X-ray Workshop S.N. Bose National Centre for Basic Sciences, 14-15/12/2011 Innovation with Integrity Overview What is the application? What are